Scanning Tunneling Microscopy with Au on Ge(111) reu/REU18/Papers/gugliada.pdf · PDF...
Embed Size (px)
Transcript of Scanning Tunneling Microscopy with Au on Ge(111) reu/REU18/Papers/gugliada.pdf · PDF...
Scanning Tunneling Microscopy with Au on Ge(111)
UC Davis REU (Dated: December 13, 2018)
The field of surface physics has become increasingly rel- evant in today’s world. It has many applications, includ- ing catalysis, corrosion, magnetic storage devices, and integrated circuits. For many decades, the electronics in- dustry has focused on decreasing the size of features on semiconductor devices, in order to increase the number of devices that can be fabricated on a silicon wafer. As the feature size decreases, it begins to approach atomic dimensions, increasing the surface area to volume ratio. In such circumstances, the study of surface physics be- comes extremely important, including processes at the atomic level.
Surface physics studies the top few atomic layers of a solid material. We are interested in understanding elec- trical contacts of metals on semiconductors. To do so, the growth of metals on semiconductors must be closely studied. Metals grow in a variety of ways on the surface of semiconductors. They may grow in flat layers, form islands, or possibly grow in nanowires. There is great interest in low-dimensional surface structures, and one- dimensional structures actually have been seen for plat- inum on germanium(001) and gold on germanium(001), where (001) is the surface structure of the germanium samples of interest.
There are many analysis methods in surface physics, including low energy electron di↵raction (LEED) and x- ray photoemission spectroscopy (XPS), among many oth- ers. This research project focused on the growth of gold on germanium(111). In order to examine these surfaces, we use a scanning tunneling microscope (STM) in an ul- trahigh vacuum (UHV) chamber. An STM can measure real space images of the sample in three dimensions.
II. TECHNICAL BACKGROUND
When Au on Ge(111) was observed with a low-energy electron microscope (LEEM), as the coverage increased, the Au grew on the surface in the Stranski-Krastanov growth mode, in which one full monolayer forms, followed by three-dimensional islands. LEEM images have shown structural phases and motion of gold islands. This STM experiment was motivated by the LEEM results, with the goal of studying this growth with the much higher spatial resolution of STM.
FIG. 1. This is the machinery in the lab. The LEEM was not
operational during the duration of this project, and the XPS
was only used for sample cleaning. All data for this project
was taken in the STM.
B. Vacuum system
The first hurdle in this research project is achieving and maintaining an ultrahigh vacuum (UHV) chamber. UHV is defined as having a pressure on the order of 10�10
torr. Since the goal is to measure the top atomic layer of a surface, it is very important that the surface accumulates as little dust as possible. At a pressure of 10�10 torr, it takes 10,000 seconds for one monolayer of dust to collect, compared to a time of only 10 seconds at 10�6 torr. Pumping the chamber down to UHV requires several
pumping stages. A roughing pump is used for some chambers, which can bring the pressure down to approx- imately 10 mtorr. A turbo pump is used after the rough- ing pump. The turbo pump can achieve a pressure on the order of 10�9 torr. Finally an ion pump can be turned on, which brings the pressure down to 10�11 torr. The vacuum chambers in the UC Davis lab are ar-
ranged as in Figure 1. Throughout the duration of this research project, the LEEM was not operational. There is an airlock chamber that allows for movement of items into and out of the STM without venting the entire cham- ber to air. The XPS was also not operational during this project, but the chamber was used for cleaning samples and deposition of metal onto samples, which will be dis- cussed in detail later. There is a gate valve between the STM and the XPS which remains closed unless a sam- ple is being moved from one chamber to the other. The transfer rod can be attached to the sample holder and is used to move the sample between chambers. The manip-
ulator has a similar purpose, which is to properly position the sample in the XPS chamber for cleaning and deposi- tion. The manipulator has external controls which allow for adjustment in the x, y, and z directions, as well as for rotating the sample about its axis.
The tunneling current is the current between the sur- face of the sample and the tungsten tip. The tip is given a bias voltage, which allows for a quantum mechanical tunneling current. For this reason, the STM can only be used to observe samples that have conducting properties. The tunneling current I is proportional to bias voltage V such that:
I / V e�A p �z, (1)
where A is a constant, � is the average work function of the tip and sample, and z is the separation between the tip and sample in Ångstroms. The tunneling current therefore has the functional form:
I / 10�z. (2)
It is then evident that the tunneling current decreases rapidly with a slight increase in separation between the tip and sample. The atom right on the end of the tip therefore has the largest contribution to the current.
The goal of these experiments is to scan the surface of samples after deposition of a metal. The first task is therefore to construct sample holders for the germanium samples.
A sample holder is displayed in Figure 2. Underneath the sample is a filament through which a current can be run. The filament then heats the sample via elec- tron beam heating, which is used for cleaning purposes. In order to measure the temperature of the sample, a chromel-alumel thermocouple is used. The sample holder is supported by four feet, and the back two are used for thermocouple wiring. One back foot is made of alumel and the other of chromel. Alumel and chromel wires are attached to their respective metal feet, and fed through the sample holder until they meet under the surface of the sample to form a thermocouple. With this arrange- ment, the temperature of the sample can be determined by the feet of the sample holder. The top plate is screwed on top of the sample to secure it.
Many di�culties in this project are due to the sam- ple holder. There are fragile parts that often need to be repaired after moving a sample holder around inside
underside exploded view
FIG. 2. This is a sample holder, which is used for securing
the sample during deposition and scanning.
FIG. 3. STM scanner placed on top of a sample.
the chambers. There is also the possibility for short cir- cuits of the thermocouple wires, which can potentially prevent a measurement of the sample temperature. An- other potential issue is a break in the filament circuit, which would prevent heating of the sample.
The scanner of the STM is placed on top of the sample, as displayed in Figure 3. A tungsten tip is inserted to the bottom of the scanner so that it is suspended just above the surface of the sample. This tip detects a tunneling current from the surface of the sample. For precision purposes, this tip must be extremely sharp, ideally one atom wide at the end. Making these tips is another major component of this project. Manufacture of the tips is done by creating the circuit
in Figure 4. As the current travels through the KOH solution, the tungsten tip is etched at the level of the solution’s meniscus. After a couple of minutes, the end of the tip falls o↵,
as seen in Figure 5. This leaves the piece of tungsten with an extremely sharp tip. While this is a fairly simple
FIG. 4. This circuit is used to create very sharp tips on pieces
of tungsten wire.
FIG. 5. The bottom of the tungsten wire eventually falls o↵,
leaving a sharp tip for use in the STM.
procedure, the tungsten wire needs to be inserted to the solution just the right amount. If it is too low, the part that falls o↵ will be too heavy and create a spring e↵ect, causing the tip to bounce up into the wire and is therefore ruined. On the other hand, if the wire is too high, the bottom part will not be heavy enough to drop o↵ and we will be left with something resembling the first part of Figure 5. It is di�cult to measure exactly how deeply the wire is suspended in the solution, but it should be only a couple of millimeters.
The sharp tip then needs to be inserted into the bottom of the scanner. This is another matter requiring precise manipulation, since the tip needs to be positioned so that it sits just above the sample surface when the scanner is placed above the sample holder. If the tip is too far down, it will crash onto the sample surface as soon as the scanner is set down. There is also the possibility of the tip being too high too get a tunneling current. There is some room for displacement in the z direction, but only a few millimeters.
FIG. 6. An evaporator is formed by a tungsten coil with
leads that can be externally connected to a power supply. A
small amount of gold is secured in the coil, which evaporates
onto the surface of the germanium sample inside the vacuum
chamber when a current is sent through.
Once there is a new germanium sample inside the STM, it must be thoroughly cleaned before deposition of another metal. To do this, we use alternating cycles of sputtering and annealing. Sputtering is the bombard- ment of the surface with argon ions. The goal of th